Accepted Manuscript Ozone and nitrogen dioxide gas sensor based on a nanostructured SrTi0.85Fe0.15O3 thin film Luís F. da Silva, Valmor R. Mastelaro, Ariadne C. Catto, Carlos A. Escanhoela Jr., Sandrine Bernardini, Sérgio C. Zílio, Elson Longo, Khalifa Aguir PII: DOI: Reference:
S0925-8388(15)00802-6 http://dx.doi.org/10.1016/j.jallcom.2015.03.089 JALCOM 33700
To appear in:
Journal of Alloys and Compounds
Received Date: Revised Date: Accepted Date:
26 November 2014 4 March 2015 10 March 2015
Please cite this article as: L.F. da Silva, V.R. Mastelaro, A.C. Catto, C.A. Escanhoela Jr., S. Bernardini, S.C. Zílio, E. Longo, K. Aguir, Ozone and nitrogen dioxide gas sensor based on a nanostructured SrTi0.85Fe0.15O3 thin film, Journal of Alloys and Compounds (2015), doi: http://dx.doi.org/10.1016/j.jallcom.2015.03.089
This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
Ozone and nitrogen dioxide gas sensor based on a nanostructured SrTi0.85Fe0.15O3 thin film Luís F. da Silva,1,2* Valmor R. Mastelaro,3 Ariadne C. Catto,3 Carlos A. Escanhoela Jr,3 Sandrine Bernardini,2 Sérgio C. Zílio,3 Elson Longo1 and Khalifa Aguir2**
1 – LIEC, Instituto de Química, Universidade Estadual Paulista, P.O. Box 355, 14800-900, Araraquara, SP, Brazil. 2 – Aix Marseille Université, CNRS IM2NP (UMR 7334), FS St Jérôme S152, Marseille, 13397, France. 3 – Instituto de Física de São Carlos, Universidade de São Paulo, Avenida Trabalhador Sãocarlense, 400, 13566-590 São Carlos, SP, Brazil.
*E-mail: [email protected]
**E-mail: [email protected]
Tel.: +55 16 33016643
Abstract In this manuscript, we report an investigation into the sensitivity of two oxidizing gases (ozone and nitrogen dioxide) for nanocrystalline SrTi0.85Fe0.15O3 thin films deposited by the electron beam physical vapor deposition technique. Annealing treatment at 500oC enhanced the crystallization and surface roughness of the thin film. Electrical measurements revealed that the thin film was sensitive to oxidizing gases, especially to low ozone gas levels, exhibiting a fast response time, a short recovery time as well as good reproducibility and reversibility. These findings demonstrate the great potential of the SrTi0.85Fe0.15O3 compound to be applied as a selective ozone gas sensor. Keywords: Perovskites; SrTi1-xFexO3; Nanostructures; Thin films; Gas sensor; Ozone; Nitrogen dioxide
Introduction Since the development of first gas detection device based on semiconducting metal
oxides, much effort has been devoted to enhancing gas sensor performance [1-5]. Nanostructured materials have drawn the interest of many researchers due to the possibility of improving the sensitivity, selectivity, response and recovery time, as well as reducing the operating sensor temperature [2-4, 6, 7]. These sensors have been widely employed in industry, agriculture and in environment control to detect reducing and oxidizing gases, such as hydrocarbons, oxygen, hydrogen (H 2), nitrogen oxides (NO2 and NOx), ammonia (NH3), sulfur dioxide (SO2), carbon monoxide (CO) and ozone (O3) [3, 8-12]. Ozone (O3) is an oxidizing gas used in important fields such as the food industry, drinking water treatment, medicine and agriculture [13-16]. Despite these important applications, ozone levels above 120 ppb become dangerous to human health, and could cause serious health problems [13, 17]. Therefore, the continuous monitoring of ozone levels present in the atmosphere is indispensable. Typical ozone gas sensors are based on SnO2, ZnO, WO3 and In2O3 compounds [7, 9, 11, 12, 18-22]. Despite the progress made, numerous studies have focused on enhancing gas sensing properties, especially selectivity [23-26]. Strontium titanate ferrite (SrTi1-xFexO3, abbreviated STFO) solid solutions are ptype semiconductors which exhibit a cubic perovskite-like structure [12, 27, 28]. The replacement of Ti4+ by Fe3+ creates negatively charged defects (Fe´Ti) [27-31], which due to the electroneutrality conditions, are compensated by the formation of oxygen vacancies (Vӧ) [28, 32]. These solid solutions have been applied as resistive gas sensors, mainly for oxygen and hydrocarbons [1, 10, 12, 31, 33-37]. As shown in Table 1, different methodologies have been employed to prepare STFO thick and/or thin films.
Insert Table 1 In recent years, our group has dedicated efforts towards investigating STFO (0.0 x 1.0) solid solutions prepared by using different synthesis routes [7, 38-40]. In an earlier study, the long- and short-range order structure and electronic properties of nanostructured STFO powders were studied . Additionally, for the first time, the ozone gas sensing properties of nanostructured STFO thin films deposited by electronbeam physical vapor deposition (EB-PVD) were also studied, looking at the influence of the Fe content on ozone gas sensing films . Despite continued progress, the gas sensing properties, particularly the sensitivity of STFO towards ozone and other analyte gases, requires further investigation. In this study, we present a detailed investigation of O3 and NO2 sensing properties of nanostructured SrTi0.85Fe0.15O3 (abbreviated as STFO15) thin films deposited by the electron beam physical vapor deposition (EB-PVD) method. The structural and microstructural properties of STFO15 samples were characterized by X-ray absorption spectroscopy (XAS) and atomic force microscopy analysis, respectively. Gas sensing properties of STFO15 thin film samples towards O3, NO2, NH3, and CO gases were evaluated, mainly concerning its selectivity. Therefore, the focus of this research was to provide a better understanding about the gas sensing properties of the nanostructured SrTi1-xFexO3 compound. 2.
Deposition of SrTi0.85Fe0.15O3 thin film and characterization techniques
The electron beam deposition technique was used for STFO15 thin film deposition. A target was produced from a nanocrystalline SrTi0.85Fe0.15O3 powder
sample synthesized via the polymeric precursor method . The STFO15 thin film, the thickness of which was monitored by a quartz balance, was deposited in a Balzers BAK600 evaporator on Si(100) and SiO2/Si substrates containing 120 nm-thick Pt electrodes. After deposition, the thin films were annealed in an electric furnace under an air atmosphere for 4 hours at 500°C with a heating rate of 5oC.min-1 . Additional details regarding the synthesis procedure of the target as well as the thin film deposition can be found in ref 27 and 40. The thin film surface microstructural characteristics were investigated using an atomic force microscope (NT-MDT SolverPro AFM) in tapping mode. The sample thickness was verified by using a field emission scanning electron microscope (FESEM, Zeiss Supra35) operating at 5 kV. The microanalysis by energy-dispersive X-ray (EDX) spectroscopy was performed in a spectrometer EDAX-AMETEC (model APPOLLO X). X-ray absorption spectroscopy (XAS) experiments were carried at the Brazilian Synchrotron
characterization technique was applied to probe the medium- and short-range order structure of STFO15 thin films deposited onto Si(100) before and after thermal treatment. Ti K-edge XANES (X-ray absorption near-edge spectroscopy) spectra were collected in fluorescence mode, at room temperature, using a 15-element Ge solid state detector (Ge-15). These spectra were recorded between 4960 and 5060 eV using an energy step of 0.3 eV around the edge. For comparison purposes among the different samples, all spectra were background removed and normalized using the first EXAFS oscillation as unity.
2.2. Gas-sensing measurements The sensing properties of nanocrystalline STFO15 film towards ozone (O 3), nitrogen dioxide (NO2), carbon monoxide (CO) and ammonia (NH3) gases were evaluated. The thin film was inserted into a special chamber which allowed for the control of the temperature and target gas concentrations. The sensor operating temperature (Topt.), which varied from 220 oC to 300oC, was maintained by an external heating source based on an Hg lamp driven by a regulated power supply. A 1 V dc voltage was applied to the thin film while the electrical resistance was monitored using an electrometer (HP4140B Source/Pico-ammeter). Dry air was used as both the reference and the carrier gas for all gases, maintaining a constant total flow of 8.3 cm3.s1
via mass flow controllers. Ozone gas was generated by oxidizing oxygen using a pen-
ray UV lamp (UVP company, model 97-0067-01), which was calibrated given an O 3 level range between 0.1 and 0.8 ppm. NO2 gas sensing measurements were performed under concentrations varying from 5 to 40 ppm. CO and NH3 gases were also employed in the range of 5 to 40 ppm. A schematic illustration of the STFO15 film based gas sensor, and a photograph of the chamber used for gas-sensing experiments are presented in Fig.1.
Insert Figure 1 The gas response or sensitivity (S) was defined as S = Rair/Rgas, where Rair and Rgas are the electric resistances of the sensor device exposed to dry air and oxidizing gases (O3 or NO2), respectively.
3. Results and Discussion 3.1. Structural and microstructural characterizations Figure 2 displays the Ti-K edge XANES spectra of the STFO15 thin film before and after thermal treatment at 500oC for 4 hours. Three transitions labeled as P1, P2, and P3 are denoted on the pre-edge region of XANES spectra. Peak P1 is related to the 1s(Ti) → 3d(t 2g)(Ti) transition, whereas P2 peak is due to the 1s(Ti) → 4p(Ti) transition, including some degree of the 1s(Ti) → 3d(eg)(Ti) quadrupole contribution.[7, 28] The P3 peak is assigned to a dipole excitation of 1s electrons to t 2g and eg orbitals of the neighboring TiO6. [28, 41] Previous results have shown that P2 intensity is directly related to Ti symmetry, exhibiting the lowest intensity for the crystalline cubic structure, whereas in noncrystalline structures it becomes more intense.  In amorphous titanate compounds, the intense P2 peak was attributed to the presence of (TiO6) and (TiO5) units. [42-45] Figure 2 inset shows a lower intensity of the P2 peak after annealing treatment, which can be attributed to an increase in (TiO6) units. Additionally, the P3 peak was visible in the spectrum of annealed sample, revealing an increase in TiO6 octahedra linkage. Likewise, the oscillations in the post-edge region (4980 to 5020 eV) were more pronounced after annealing. These three effects caused by annealing can be interpreted as an increase in the short and medium range-order around titanium atoms, allowing for the conclusion that the degree of crystallization of the STFO15 sample increased after annealing.
Insert Figure 2 Figure 3 shows the AFM images of the STFO15 thin film before and after annealing at 500oC. Before annealing, the sample exhibited a flat surface with an Rrms (root-mean-square) roughness around 0.748 nm. After annealing, the sample presented a
microstructure characteristic of nanocrystalline thin films exhibiting grain sizes between 30 and 150 nm and an Rrms around 4.0 nm.
Insert Figure 3
Figure 4 shows the EDX spectra of the STFO15 ceramic pellet (used as target) and STFO15 thin film after annealing treatment. The EDX spectra detected the presence of Sr, Ti, Fe, and O elements in both samples, whereas the Si peak was observed only for the thin film. Additionally, the (Sr+Ti)/Fe ratio was approximately 1.2 (ceramic pellet) and 1.4 (thin film), suggesting that the stoichiometry of the STFO15 thin film was preserved during the deposition process.
Insert Figure 4 3.2. Gas sensing properties First, the electrical resistance of the STFO15 thin film before annealing exhibited a higher resistivity, due the presence of several porous (see Fig. 3b), resulting in a low densification of the sample. The electrical resistance of the STFO15 thin film annealed at 500oC presented typical values of metal oxide semiconductor sensors and was then monitored when exposed to 0.8 ppm of O3 (Fig. 6a) and 40 ppm of NO2 (Fig. 6b) for various periods of time at an operating temperature of 260oC for O3 and 220oC for NO2. As can be seen, the gas sensor response of the STFO15 thin film was characteristic of a p-type semiconductor. In addition, the STFO15 thin film showed good sensitivity, even for short periods of time, total reversibility and good stability of the baseline toward O3 and NO2 gases. For NO2 gas, it was observed that the sample reached a saturation level at times longer than 30 s.
Insert Figure 5
It is well-established that the detection of oxidizing gases on a p-type sensor material is based on the surface adsorption of the gas molecules, leading to the formation of a hole-accumulation layer which causes an increase in the current density. [4, 46, 47] The gas sensor response of the STFO15 thin film for these two oxidizing gases (O3 and NO2) can be explained by the follow reactions: [18, 46]
To determine the optimum operating temperature (Topt), the annealed STFO15 thin film was exposed for 30 s to 0.8 ppm of O3 and afterwards to 40 ppm of NO2. The results presented in Fig. 6 show a maximum sensitivity value at 260oC for both target gases, which is close to that of traditional metal oxide gas sensors such as WO 3, In2O3, and SnO2.[9, 11, 12, 19, 20, 46, 48] Chan and co-workers synthesized STFO thin films via a sol-gel spin-coating method and applied them as oxygen gas sensors, with an operating temperature ranging around of 350oC for an iron content of x= 0.2.  On the other hand, STFO thick films obtained via solid-state reaction method exhibited good gas sensing performance towards oxygen at temperatures above 600oC.[33, 34, 36, 50]
Insert Figure 6 Based on the above results, the STFO15 thin film was kept at 260oC and then exposed for 30 s to different O3 levels (0.1 to 0.8 ppm). As can be seen in Fig. 7, it is
noteworthy that the film displayed good sensitivity even at lower O 3 levels, total reversibility, as well as good reproducibility. In addition, the response time varied from 26 s (0.1 ppm) to 28 s (0.8 ppm), while the recovery time varied from 72 s (0.1 ppm) to 161 s (0.8 ppm). Although the response time (tres) for STFO15 thin film was greater than for WO3 compound (tres ~ 1 s), the recovery time (trec) was relatively shorter (trec < 60 s) 
Insert Figure 7 In a similar procedure, the annealed STFO15 thin film was also kept at 260oC and exposed to NO2 gas. As depicted in Fig. 8, even at 5 ppm NO2, the material showed a noticeable response as well as good reproducibility and reversibility.
Insert Figure 8 Gas sensing experiments were also performed using the carbon monoxide (CO) and ammonia (NH3) gases. The STFO15 thin film did not exhibit any sensitivity to these gases in the range of 5 to 40 ppm when measured at different operating temperatures (220-300oC). Figures 9(a) and 9(b) show the sensitivity values of the annealed STFO15 thin film as function of O3 and NO2 concentrations, respectively, at a working temperature of 260oC. In the case of O3 gas, the sensitivity increased with the gas concentration, reaching a saturation level above 0.6 ppm, whereas for NO2 gas, the saturation level was not reached even at the highest concentration allowed by the mass flux controller.
Insert Figure 9 Gas selectivity is one of the most important parameters and also a challenge for the manufacture of metal-oxide gas sensor devices. [2, 4, 51] Figure 10 displays the comparison of the sensitivity values of the annealed STFO15 thin film when exposed to oxidizing (O3 and NO2) and reducing (CO and NH3) gases at 260oC. In order to further
exploit the selectivity of the film, we chose similar gas concentrations, i.e., 0.8 ppm O3 and 5 ppm NO2, to compare the gas sensing performance. As can be seen, the annealed STFO15 thin film showed the highest sensitivity to O3 (19.8) when compared to NO2 (4.3) and non-detectable sensitivity to CO and NH3 gases. Based on these findings, we can state that the STFO15 thin film can be considered as a promising material for an ozone gas sensor.
Insert Figure 10 4. Conclusions We have successfully obtained nanocrystalline SrTi0.85 Fe0.15O3 thin films via the electron beam deposition technique. X-ray absorption spectroscopy measurements showed that the annealing treatment was effective in increasing the degree of crystallization of the STFO15 thin film, which led to an increase in surface roughness, according to AFM analysis. Electrical resistance measurements pointed out the good sensitivity, fast response and short recovery time of the annealed STFO15 thin film when exposed to O3 and NO2 oxidizing gases. Due to the good sensing properties to ozone gas, this material can be considered as a promising material for ozone gas sensors.
5. Acknowledgments The authors are grateful for the financial support from the Brazilian research funding institution CNPq (MCT/CNPq, under grants No. 70/2008 and 150753/2013-6) and FAPESP (under grants No. 2013/09573-3, 2013/07296-2, 2013/12473-0 and 2012/15170-6). This research was partially performed at the Brazilian Laboratory of Synchrotron Radiation (LNLS) and the Brazilian Nanotechnology National Laboratory (LNNano), Microfabrication laboratory (Project 17168), Campinas, SP, Brazil.
A. Rothschild, H.L. Tuller, J. Electroceram. 17 (2006), 1005-1012.
G. Jimenez-Cadena, J. Riu, F.X. Rius, Analyst 132 (2007) 1083-1099.
G. Korotcenkov, Handbook of Gas Sensor Materials: Properties, Advantages and Shortcomings for Applications New York: Springer; 2013.
H.-J. Kim, J.-H. Lee, Sens. Actuators B 192 (2014) 607-27.
L.F. da Silva, A.C. Catto, W. Avansi, L.S. Cavalcante, J. Andres, K. Aguir, V. R. Mastelaro, E. Longo, Nanoscale 6 (2014) 4058-4062.
K. Sahner, M. Kaspar, R. Moos, Sens. Actuators B 139 (2009) 394-399.
A.C. Catto, L.F. da Silva, M.I.B. Bernardi, M.S. Li, E. Longo, P.N. Lisboa-Filho, O R. Nascimento, V.R. Mastelaro, J Nanopart Res, 16 (2014) 1-9.
P. Meuffels, J. Europ. Ceram. Soc. 27 (2007) 285-290.
K. Aguir, C. Lemire, D.B.B. Lollman, Sens. Actuators B 84 (2002) 1-5.
G. Neri, G. Micali, A. Bonavita, R. Licheri, R. Orrù, G. Cao, D. Marzorati, E. Merlone Borla, E. Roncari, A. Sanson, Sens. Actuators B 134 (2008) 647-53.
M. Bendahan, R. Boulmani, J.L. Seguin, K. Aguir, Sens. Actuators B 100 (2004) 320324.
S.J. Litzelman, A. Rothschild, H.L. Tuller, Sens. Actuators B 108 (2005) 231-237.
L.C. Simoes, M. Simoes, RSC Adv. 3 (2013) 2520-2533.
S. Patil, P. Bourke, J.M. Frias, B.K. Tiwari, P.J. Cullen, Innovative Food Sci. Emerging Technol. 10 (2009) 551-557.
H.-P. Kaiser, O. Koester, M. Gresch, P.M.J. Perisset, P. Jaeggi, E. Salhi, et al., Ozone: Sci. Eng. 35 (2013) 168-185.
L.S. Hansen, P. Hansen, K.M.V. Jensen, J. Stored Prod. Res. 54 (2013) 59-63.
C.Y. Wang, R.W. Becker, T. Passow, W. Pletschen, K. Köhler, V. Cimalla, O. Ambacher, Sens. Actuators B 152 (2011) 235-240.
M. Acuautla, S. Bernardini, L. Gallais, T. Fiorido, L. Patout, M. Bendahan, Sens. Actuators B 203 (2014) 602-611.
A.C. Catto, L.F. da Silva, C. Ribeiro, S. Bernardini, K. Aguir, E. Longo, V.R. Mastelaro, RSC Adv. 5 (2015) 19528-19533.
G. Korotcenkov, B.K. Cho, Sens. Actuators B 161 (2012) 28-44.
D. Barreca, D. Bekermann, E. Comini, A. Devi, R.A. Fischer, A. Gasparotto, C. Maccato, C. Sada, G. Sberveglieri, E. Tondello, Crystengcomm, 12 (2010) 3419-3421.
A. Gurlo, Nanoscale 3(2011) 154-165.
T. Xiao, X.Y. Wang, Z.H. Zhao, L. Li, L. Zhang, H.C. Yao, J.S. Wang, Z.J. Li, Sens. Actuators B 199 (2014) 210-219.
Q. Simon, D. Barreca, A. Gasparotto, C. Maccato, E. Tondello, C. Sada, E.Comini, A. Devi, R.A. Fischer, Nanotechnol. 23 (2012) 025502.
A. Sharma, M. Tomar, V. Gupta, Sens. Actuators B 181(2013) 735-742.
X.T. Yin, X.M. Guo, Sens. Actuators B 200 (2014) 213-218.
L.F. da Silva, J.-C. M’Peko, J. Andrés, A. Beltrán, L. Gracia, M.I.B. Bernardi, A. Mesquita, E, Antonelli, M.L. Moreira, V.R. Mastelaro, J. Phys. Chem. C 118 (2014) 4930-4940.
M. Vračar, A. Kuzmin, R. Merkle, J. Purans, E.A. Kotomin, J. Maier, O. Mathon, Phys. Rev. B 76 (2007) 174107.
A. Rothschild, W. Menesklou, H.L. Tuller, E. Ivers-Tiffee, Chem. Mater. 18 (2006) 3651-3659.
E. Blokhin, E. Kotomin, A. Kuzmin, J. Purans, R. Evarestov, J. Maier, Appl. Phys. Lett. 102 (2013) 112913.
A. Rothschild, S.J. Litzelman, H.L. Tuller, W. Menesklou, T. Schneider, E. Ivers-Tiffée, Sens. Actuators B 108 (2005) 223-230.
L.H. Brixner, Mater. Res. Bull. 3 (1968) 299-308.
G. Neri, A. Bonavita, G. Micali, G. Rizzo, R. Licheri, R. Orrù, G. Cao, Sens. Actuators B 126 (2007) 258-265.
A. Sanson, E. Mercadelli, E. Roncari, R. Licheri, R. Orrù, G. Cao, E. Merlone-Borla, D.Marzorati, A. Bonavita, G. Micali, G. Neri. Ceram. Int. 36 (2010) 521-527.
S.-H. Choi, S.-J. Choi, B.K. Min, W.Y. Lee, J.S. Park, I.-D. Kim, Macromol. Mater. Eng. 298 (2013) 521-527.
G. Jin, G. Choi, W. Lee, J. Park, J. Nanosci. Nanotechnol. 11(2011) 1738-1741.
W. Lee, D. Na, J. Park, J. Ceram. Process. Res. 13 (2012) 717-720.
L.F. da Silva, W. Avansi, Jr., M.L. Moreira, J. Andres, E. Longo, V.R. Mastelaro, Crystengcomm, 14 (2012) 4068-4073.
V.R. Mastelaro, S.C. Zílio, L.F. da Silva, P.I. Pelissari, M.I.B. Bernardi, J. Guerin, K. Aguir, Sens. Actuators B 181 (2013) 919-924.
L.F. da Silva, M.I.B. Bernardi, L.J.Q. Maia, G.J.M. Frigo, V.R. Mastelaro, J. Therm. Anal. Calorim. 97 (2009) 173-177.
R.V. Vedrinskii, V.L. Kraizman, A.A. Novakovich, P.V. Demekhin, S.V. Urazhdin, J. Phys.: Condens. Matter 10(1998) 9561-9580.
V.M. Longo, A.T. de Figueiredo, S. de Lazaro, M.F. Gurgel, M.G.S. Costa, C.O. PaivaSantos, J.A. Varela, E. Longo, V.R. Mastelaro, F.S. deVicente, A.C. Hernandes, R.W.A. Franco, J. Appl. Phys. 104 (2008) 023515.
A.T. de Figueiredo, V.M. Longo, R.O. da Silva, V.R. Mastelaro, A. Mesquita, R.W.A. Franco, J.A. Varela, E. Longo, Chem. Phys. Lett. 544 (2012) 43-48.
A.T. de Figueiredo, V.M. Longo, S. de Lazaro, V.R. Mastelaro, F.S. De Vicente, A.C. Hernandes, M.S. Li, J.A. Varela, E. Longo, J. Luminescence 126 (2007) 403-407.
S. de Lazaro, J. Milanez, A.T. de Figueiredo, V.M. Longo, V.R. Mastelaro, F.S. De Vicente, J. A. Varela, E. Longo, Appl. Phys. Lett. 90 (2007) 111904.
S. Maeng, S.-W. Kim, D.-H. Lee, S.-E. Moon, K.-C. Kim, A. Maiti, ACS Appl. Mater. Interf. 6 (2013) 357-363.
D. Peeters, D. Barreca, G. Carraro, E. Comini, A. Gasparotto, C. Maccato, C. Sada, G. Sberveglieri, J. Phys. Chem. C 118(2014) 11813-11819.
G. Korotcenkov, V. Macsanov, V. Tolstoy, V. Brinzari, J. Schwank, G. Faglia, Sens. Actuators B 96 (2003) 602-609.
C.L. Chow, W.C. Ang, M.S. Tse, O.K. Tan, Thin Solid Films 542 (2013) 393-398. W. Menesklou, H.-J. Schreiner, K.H. Härdtl, E. Ivers-Tiffée, Sens. Actuators B 59 (1999) 184-189.
A. Gurlo, R. Riedel, Angew. Chem. Int. Ed. 46 (2007) 3826-3848.
Table 1. Brief summary of results reported for SrTi1-xFexO3 compounds prepared by various methodologies applied as resistive gas sensors towards various target gases.
Figure 1. Preparation and gas-sensing tests of the gas sensor device. (a) Schematic structure of the sensor device. (b) Photograph of the gas sensor test chamber.
Figure 2. Ti-K edge spectra of STFO15 thin film before and after annealing at 500oC for 4 hours. The inset shows the pre-edge region of XANES spectra.
Figure 3. AFM images of STFO15 thin film (a) before and (b) after annealing treatment at 500oC for 4 hours.
Figure 4. Energy dispersive X-ray (EDX) spectroscopy analysis of the (a) STFO15 ceramic pellet and (b) STFO15 thin film annealing treated at 500oC.
Figure 5. Gas sensing response of the STFO15 thin film exposed for different times: (a) 0.8 ppm O3 at 260oC and (b) 40 ppm NO2 at 220oC. Figure 6. Gas sensor response of the STFO15 thin film exposed to 0.8 ppm O 3 and 40 ppm NO2 at different operating temperatures.
Figure 7. Ozone gas sensing response for the STFO15 thin film as a function of the gas level at an operating temperature of 260oC. Figure 8. NO2 gas sensing responses for STFO15 thin film at 260oC for various NO2 levels (5-40 ppm). Figure 9. Sensitivity versus gas concentration in the range (a) 0.1 – 0.8 ppm O3 and (b) 5 – 40 ppm NO2. Figure 10. Gas sensor response of the STFO15 thin film to oxidizing (O3 and NO2) and reducing (CO and NH3) gases at an operating temperature of 260oC.
Tables Table 1
Operating Temp. (oC)
Mixed oxides reaction
O2, NO, NO2, CO, CO2 ,CH4
Mixed oxides reaction
Pulsed laser deposition
Mixed oxides reaction
Self-propagating hightemperature reaction
Nanostructured SrTi1-xFe xO3 films were deposited by electron beam evaporation.
XANES spectroscopy revealed an increase of crystallization after heattreatment.
Annealing treatment contributes improving the gas-sensing performance.
The SrTi1-xFe xO3 film exhibited a good sensitivity to oxidizing gases.
The results show that SrTi1-xFe xO3 can be considered a potential ozone gas sensor.